- Nano Express
- Open Access
Semiconductor Gas Sensors Based on Pd/SnO2 Nanomaterials for Methane Detection in Air
© The Author(s). 2017
Received: 18 October 2016
Accepted: 24 April 2017
Published: 4 May 2017
Semiconductor sensors based on nanosized Pd-containing tin dioxide have been obtained by a sol–gel technique. Semiconductor gas-sensitive materials were characterized by transmission electron microscopy (TEM) and X-ray diffraction (XRD) methods. Influence of Pd additives on sensitivity of the sensors to methane has been studied. Temperature dependences of electrical resistance in air and sensor response to methane on palladium content for the sensors based on nanosized materials Pd/SnO2 have been investigated.
Natural gas is one of the main energy sources nowadays. Even the development of alternative energy could not deliver from necessity of its usage, because methane, the main component of the natural gas, is widely used in industry. Methane can combine with air explosively and is one of the greenhouse gasses. That is why, its leakages are extremely dangerous from both economy and ecology point of views. Thus, the natural gas detection is an actual problem. Different types of detectors are used for its solving [1–5]. Adsorption-semiconductor sensors are quite promising among them because of their high sensitivity, low power consumption, and small weight and sizes.
Response of the semiconductor sensor is determined by a change in chemisorbed oxygen quantity on a surface of a gas-sensitive layer in the presence of an analyzed gas. Heterogeneous catalytic oxidation of the analyzed gas takes place on the surface and leads to the chemisorbed oxygen decreasing. This change in the semiconductor surface layer causes charge carrier quantity to increase in the valence band of the semiconductor that leads to a decrease in electrical resistance .
The sensitivity of the adsorption-semiconductor sensors can be enhanced by increasing a rate of the analyzed gas oxidation. It can be attained by addition of catalytic active dopants. In this study, nanosized tin dioxide doped by palladium has been chosen as a gas-sensitive sensor material. Tin dioxide is known to be a chemically inert semiconductor material, and palladium is known to be one of the best methane combustion catalysts.
The aim of the study was to create adsorption-semiconductor sensors highly sensitive to CH4 based on Pd/SnO2 and investigate their properties.
Nanosized tin dioxide with particle sizes 10–11 nm (obtained as described in [7, 8]) was mixed with a colloid solution of carboxymethyl cellulose to form a creamy-like paste. The paste was applied on a plate (size 2.2 mm × 2.2 mm × 0.5 mm) of the sensor (the sensor construction was presented in ). The next step was a drying of the sensor plates in air at 90 °C during 1 h to remove excess of water. Palladium was added to the paste by a wet impregnation technique using PdCl2 solutions. The concentrations of the solutions were varied from 0.21 × 10−2 to 35 × 10−2 mol/L PdCl2. After impregnation, the sensor plates were dried at 90 °C and then were sintered in the temperature range 20–620 °C in air to form the gas-sensitive layers of the sensors. Gas-sensitive materials and sensors based on the materials were prepared by the same procedure.
Morphology of the initial obtained nanomaterials and the gas-sensitive layer materials was studied by TEM using SELMI PEM-125K (Selmi, Ukraine) with accelerating voltage of 100 kV. For TEM study, the samples were previously dispersed in ethanol by ultrasonic treatment during 10 min. The obtained colloid solution was dropped onto a copper mesh with amorphous carbon film transparented for electron beam. Vacuum in a chamber of the TEM reached to 10−4 Pa. Particle size distribution analysis was performed using ImageJ software.
Contents of palladium in the sensor materials were determined by X-ray fluorescence analysis using an energy dispersion X-ray spectrometer ElvaX EXS - 01 (Elvatech, Ukraine).
Catalytic Activity Measurement
Catalytic activity of the Pd/SnO2 materials was studied in a flow-type reactor using methane–air mixture (937 ppm CH4) with a flow rate 50 ml/min. Analysis of the gas mixture components was performed by a chromatographic method using a flame ionization detector (Shimadzu GC-14, Japan). The weight of the analyzed catalyst was 200 mg. The temperature of the 10% methane conversion (T 10) was taken as a measure of the catalytic activity of the samples.
Sensor Characteristic Measurement
The sensors were aged for stabilization of their electric characteristics before measurement of the sensor response to methane. In particular, they were periodically treated by methane–air mixture (937 ppm CH4) for 30 s per 1 h at 405 °C during 3 days.
Temperatures of the gas-sensitive layers of the sensors were measured by an infrared radiation pyrometer Optris LaserSight (Optris, Germany).
A measure of the sensor response was taken as a ratio R 0/R CH4, where R 0 is a value of electric resistance of the sensor in air and R CH4 is a value of electric resistance in the mixture of air with 937 ppm of CH4. The gas mixture was prepared in gas balloons under pressure and certified at the Ukrainian Center of Certification and Metrology. Methane–air mixtures with lower CH4 concentrations (from 47 to 937 ppm) obtained through dilution generators were used to study dependence of the sensor signal on CH4 concentration.
To determine a value of the signal of the sensor, it was placed into a chamber and heated up in air to a definite temperature in a range of 225–405 °C. Then, the chamber was flown by air or by analyzed methane–air mixture until a constant value of the detected sensor signal had been set. The rates of flows of air and the methane–air mixture were the same and equal to 400 ml/min.
Two parameters of the sensors (response time (τ 0.9) and recovery time (τ relax)) were used to estimate dynamic properties of the sensors. A value τ 0.9 was estimated as a time required for the sensor signal to reach 90% of its equilibrium value through an injection of the analyzed gas. The recovery time (τ relax) was estimated as a time necessary for the sensor to return to 10% above the initial sensor signal in air after the analyzed gas has been released.
Results and Discussion
Particle sizes of SnO2-based sensor nanomaterials obtained by TEM and calculated by XRD data
TEM size, nm
XRD size, nm
Initial tin dioxide
Sensor material without Pd
It should be noted that electrical resistance of the sensors depends greatly on chemisorbed oxygen content. Chemisorbed oxygen species are negatively charged due to localization at chemisorbed oxygen of electrons from the semiconductor conduction band, and such process formed negatively charged surface potential. Thus, the near-surface layer of the semiconductor becomes depleted by electrons due to the presence of such a potential . In the process of high-temperature formation of the sensor nanomaterial, many intergrain contacts are formed. Due to the presence of the negatively charged surface potential on each grain boundary, a lot of potential barriers are formed and they impede a directed movement of electrons in the material of the gas-sensitive layer of the sensor under an electric field action [22, 23]. As a result, a value of the electrical resistance of the sensor in air (R 0) increases.
The potential barrier plays a dominant role in forming the resistance of the sensor (R), and when all other conditions of the sensor operation are equal (nature of the sensitive material, temperature of the sensor, etc.), a height of the potential barrier is determined by the quantity of the chemisorbed oxygen on the surface of the sensor. When the sensor is placed in air at very high temperatures, the desorption of the chemisorbed oxygen occurs [18, 19, 24], and thus, the quantity of the chemisorbed charged oxygen species decreases. This process leads to a decrease in the height of the potential barrier and an increase in the concentration of the main charge carriers in the near-surface layer of the semiconductor [21, 23]. The desorption of oxygen leads to a decrease in the sensor resistance.
In the presence of CH4, a chemical reaction of methane with active charged forms of oxygen occurs on the surface of the heated sensor and, as a result, the quantity of the chemisorbed charged oxygen forms decreases. Such oxygen decreasing leads also to a decrease in the height of the potential barrier in the near-surface layer of the semiconductor, and thus, the electrical resistance of the sensor decreases. A rate of CH4 catalytic oxidation and thus a quantity of oxygen chemisorbed on the sensor surface which takes part in the oxidation reaction depends on the methane concentration in air. The higher is the CH4 concentration the faster is the rate of the oxidation and the higher quantity of oxygen will take part in the oxidation reaction. As a result, a more significant decreasing in the electrical resistance of the sensor will be observed.
Concerning the temperature dependences of the sensor responses, as can be seen from Fig. 3a, b, the responses to CH4 for the sensors with a low content of palladium (0.087–0.31% Pd) increases with increasing temperature. The temperature dependences of the responses to methane for sensors with a high content of palladium (0.62–3.31% Pd) are extreme. Such characters of the observed temperature dependences are determined by the effect of adsorption and desorption of oxygen which takes part in the heterogeneous catalytic oxidation of methane on the surface of the sensor. It should be noted that for the sensors with palladium content more than 0.62% Pd, an increase of weakly bounded oxygen can promote a shift in the maximum of the sensor response to the region of the lower sensor temperatures as it was found for the electrical resistance of the sensors. Thus, the maximum of the responses for the sensors with 0.087–0.31% Pd could be located above 400 °C (nonexplored temperature region), but for the sensors containing 0.62% Pd, the maximum have already been observed at 350–380 °C (Fig. 3).
The highest electrical resistance was found for the sensors based on 1.41% Pd/SnO2 at 290 °C so the longest interface palladium–tin dioxide could be supposed for this material. Thus, the highest response to methane should be observed for the sensors with 1.41% Pd, and it was found experimentally (Fig. 3). Further increase in Pd content leads to aggregation of the palladium particles and decreases the interface length. As a result, the response and electrical resistance of the sensors based on semiconductor material with higher palladium content are lower (Figs. 3 and 4).
It should be noted that the temperature which corresponded to the maximum of the sensor response is shifted (~40–80 °C) to higher temperature in comparison with the temperature which corresponded to the maximum of the electrical resistance in air for the sensors based on the same material (Figs. 3 and 4). This shift can arise due to the factors affecting the values of the sensor electrical resistances in air and sensor response in the presence of methane at a definite sensor temperature. The value of the sensor resistance in air depends on the quantity of the chemisorbed oxygen on the sensor surface. In the presence of methane, the sensor response depends on the rate of the catalytic oxidation of CH4 on the gas-sensitive layer of the sensor. This rate will depend not only on the quantity of the chemisorbed oxygen but also on the temperature activation of methane that will increase significantly the oxidation rate of CH4 and hence the sensor response to methane. It is known that temperature activation of CH4 in its oxidation reaction requires high temperature for deposited systems (e.g., Pd/Al2O3, Pd/SiO2, Pd/SnO2) [12, 26, 27]. That is why, the temperature shift of the maximum of the sensor responses to methane in comparison with the maximum of their resistances becomes especially noticeable at relatively high temperatures (350–380 °C) of the sensor (Fig. 3) when the temperature activation of methane can be achieved. The effect of such activation is confirmed by the data in , where the high catalytic activity of deposited systems Pd/SnO2 in the methane oxidation reaction was achieved at high temperatures and by our data for the created Pd/SnO2 sensor nanomaterials also. In particular, it was found that the catalytic activities of the obtained Pd/SnO2 sensor nanomaterials were only observed at high catalyst temperatures (10% methane conversion is achieved at temperatures of 358–474 °C). Besides, it is known that chemical interaction of methane with charged forms of chemisorbed oxygen affects the conductivity of tin dioxide and the presence of two forms of palladium is necessary for the catalytic reaction of CH4 oxidation in the palladium-containing deposited systems . XPS study of the obtained Pd/SnO2 sensor nanomaterial showed a presence of two forms of palladium with binding energies of 335.5 and 337.5 eV (Pd0 and Pd2+) , which caused the activities of Pd/SnO2 sensor materials in the methane oxidation reaction and, as a result, the high responses to methane of the sensors created on their base.
Perspectives of using the adsorption-semiconductor sensors based on nanosized Pd/SnO2 have been shown for methane detection in air. Addition of palladium in tin dioxide significantly increases the sensor response to methane (in ~6–7 times) in comparison with nondoped materials. The dependences of the electrical resistance in air and sensitivity to CH4 of the sensors with different palladium contents at different sensor temperatures were explained by an interaction between methane and oxygen chemisorbed on the interface between palladium particles and tin dioxide support. The created sensors can measure methane in a wide range of its concentration and demonstrate a fast response and recovery time.
LO and NM conceived and designed the experiment. GF synthesized the nanomaterials. OR created the sensors. GF and GS provided the sensors’ measurements. LO, NM, and GF wrote the paper. All authors read and approved the final manuscript.
The authors declare that they have no competing interests.
Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Open AccessThis article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.
- Ho CK, Itamura MT, Michael K, Hughes RC (2001) Review of chemical sensors for in-situ monitoring of volatile contaminants. Sandia ReportView ArticleGoogle Scholar
- Mine Safety Appliances Company (MSA). Gas detection handbook. 5th ed. USA: MSA; 2007. http://www.gilsoneng.com/reference/gasdetectionhandbook.pdf.
- Wawrzyniak R, Wasiak W (2011) Chromatographic, spectrophotometric and electrochemical methods in determination of biogas component. Ecological Chem Eng S 18(4):537–544Google Scholar
- Wang Z, Xiaoyi M, Guo M et al (2013) Methane recognition and quantification by differential capacitance at the hydrophobic ionic liquid-electrified metal electrode interface. J Electrochem Soc 160(6):B83–B89View ArticleGoogle Scholar
- Wang Z, Guo M, Baker GA et al (2014) Methane–oxygen electrochemical coupling in an ionic liquid: a robust sensor for simultaneous quantification. Analyst 139:5140–5147View ArticleGoogle Scholar
- Miller TA, Bakrania SD, Perez C, Wooldridge MS (2006) Nanostructured tin dioxide materials for gas sensor applications. In: Kurt E. Geckeler, Edward Rosenberg (eds) Functional Nanomaterials. Valencia: American Scientific Publishers; 515.Google Scholar
- Zhang G, Liu M (1999) Preparation of nanostructured tin oxide using a sol–gel process based on tin oxide a sol–gel process based on tin tetrachloride and ethylene glycol. J Mat Sci 34:3213–3219View ArticleGoogle Scholar
- Sokovykh EV, Oleksenko LP, Maksymovych NP, Matushko IP (2015) Influence of temperature conditions of forming nanosized SnO2-based materials on hydrogen sensor properties. J Therm Anal Calorim 121:1159–1165View ArticleGoogle Scholar
- Vorotyntsev V, Maksimovich N, Yeremina L, Kaskevich O, Nikitina N (1996) Adsorption semiconductor gas sensors and heterogeneous catalytic reaction mechanisms. Sens Actuators B Chem 35–36:333–337View ArticleGoogle Scholar
- Hammond C (2009) The basics of crystallography and diffraction. Oxford Univ. Press, OxfordGoogle Scholar
- Fedorenko GV, Oleksenko LP, Maksymovych NP, Matushko IP (2015) Semiconductor adsorption sensors based on nanosized Pt/SnO2 materials and their sensitivity to methane. Russ J Phys Chem 12:2259–2262View ArticleGoogle Scholar
- Takeguchi T, Takeoh O, Aoyama S, Ueda J, Kikuchi R, Eguchi K (2003) Strong chemical interaction between PdO and SnO2 and the influence on catalytic combustion of methane. Appl Catal A Gen 252:205–214View ArticleGoogle Scholar
- Borchert H, Shevchenko EV, Robert A et al (2005) Determination of nanocrystal sizes: a comparison of TEM, SAXS, and XRD studies of highly monodisperse CoPt3 particles. Langmuir 21:1931–1936View ArticleGoogle Scholar
- Vasylenko IV, Kolotilov SV, Kotenko IE, Gavrilenko KS, Tuna F, Timco GA, Winpenny REP, Pavlishchuk VV (2012) Magnetic properties of nanosized γ-Fe2O3 and α-(Fe2/3Cr1/3)2O3, prepared by thermal decomposition of heterometallic single-molecular precursor. J Magn Magn Mater 324:595–601View ArticleGoogle Scholar
- Kappler J, Barsan N, Weimar U, Dièguez A, Alay JL, Romano-Rodriguez A, Morante JR, Göpel W (1998) Correlation between XPS, Raman and TEM measurements and the gas sensitivity of Pt and Pd doped SnO2 based gas sensors. Fresenius J Anal Chem 361:110–114View ArticleGoogle Scholar
- Green IX, Tang W, Neurock M, Yates JT (2011) Spectroscopic observation of dual catalytic sites during oxidation of CO. Science 333:736–739View ArticleGoogle Scholar
- Jaramillo TF, Jorgensen KP, Bonde J et al (2007) Identification of active edge sites for electrochemical H2 evolution from MoS2 nanocatalysts. Science 317:100–102View ArticleGoogle Scholar
- Kang WP, Kim CK (1994) Performance analysis of a new metal–insulator–semiconductor capacitor incorporated with Pt–SnO x catalytic layers for the detection of O2 and CO gases. J Appl Phys 75:4237–4242View ArticleGoogle Scholar
- Cabot A, Arbiol J, Morante JR, Weimar U, Barsan N, Gopel W (2000) Analysis of the noble metal catalytic additives introduced by impregnation of as obtained SnO sol–gel nanocrystals for gas sensors. Sens Actuators B Chem 70:87–100View ArticleGoogle Scholar
- Barsan N, Weimar U (2001) Conduction model of metal oxide gas sensors. J Electroceram 7:143–167View ArticleGoogle Scholar
- Marikutsa AV, Rumyantseva MN, Gaskov AM, Samoylov AM (2015) Nanocrystalline tin dioxide: basics in relation with gas sensing phenomena. Part I. Physical and chemical properties and sensor signal formation. Inorg Mater 51:1329–1347View ArticleGoogle Scholar
- Yamazoe N, Shimanoe K (2009) New perspectives of gas sensor technology. Sensors Actuators B 138:100–107View ArticleGoogle Scholar
- Yamazoe N, Shimanoe K (2008) Theory of power laws for semiconductor gas sensors. Sensors Actuators B 128:566–573View ArticleGoogle Scholar
- Oleksenko LP, Maksymovych NP, Buvailo AI, Matushko IP, Dollahon N (2012) Adsorption-semiconductor hydrogen sensors based on nanosized tin dioxide with cobalt oxide additives. Sens Actuators B Chem 174:39–44View ArticleGoogle Scholar
- Chou P, Albert Vannice M (1987) Calorimetric heat of adsorption measurements on palladium. J Catal 105:342–351View ArticleGoogle Scholar
- Burch R, Hayes MJ (1995) C-H bond activation in hydrocarbon oxidation on solid catalysts. J Mol Catal A Chem 100:13–33View ArticleGoogle Scholar
- Persson K, Ersson A, Jansson K, Iverlund N, Järås S (2005) Influence of co-metals on bimetallic palladium catalysts for methane combustion. J Catal 231:139–150View ArticleGoogle Scholar
- Fujimoto K-I, Ribeiro FH, Avalos-Borja M, Iglesia E (1998) Structure and reactivity of PdOx/ZrO2 catalysts for methane oxidation at low temperatures. J Catal 179:431–442View ArticleGoogle Scholar
- Sokovykh EV, Oleksenko LP, Maksymovych NP et al (2012) Study of influence of palladium additives in nanosized tin dioxide on sensitivity of adsorption semiconductor sensors to hydrogen. Chemistry, Physics Technol Surface 3:312–316Google Scholar
- Chakraborty S, Sen A, Maiti HS (2006) Selective detection of methane and butane by temperature modulation in iron doped tin oxide sensors. Sensors Actuators B 115:610–613View ArticleGoogle Scholar
- Cirera A, Cabot A, Cornet A, Morante JR (2001) CO – CH4 selectivity enhancement by in situ Pd – catalysed microwave SnO2 nanoparticles for gas detectors using active filter. Sens Actuators B Chem 78:151–160View ArticleGoogle Scholar
- Quaranta F, Rella R, Siciliano P, Capone S, Epifani M, Vasanelli L, Licciulli A, Zocco A (1999) A novel gas sensor based on SnO2/Os thin film for the detection of methane at low temperature. Sens Actuators B Chem 58:350–355View ArticleGoogle Scholar
- Bose S, Chakraborty S, Ghosh BK, Dasc D, Sena A, Maiti HS (2005) Methane sensitivity of Fe-doped SnO2 thick films. Sens Actuators B Chem 105:346–350View ArticleGoogle Scholar
- Papadopoulos CA, Vlachos DS, Avaritsiotis JN (1996) Comparative study of various metal-oxide-based gas-sensor architectures. Sens Actuators B Chem 32:61–69View ArticleGoogle Scholar
- Sun L, Qiu F, Quan B (2000) Investigation of a new catalytic combustion-type CH4 gas sensor with low power consumption. Sens Actuators B 66:289–292View ArticleGoogle Scholar
- Abbaszadeha D, Ghasempoura R, Rahimi F, Iraj zad A (2006) Effective factors on methane sensing of tin-oxide activated by palladium in sol–gel process. Sens Transducers J 73:819–825Google Scholar
- Wagner T, Bauer M, Sauerwald T, Kohl C-D, Tiemann M (2011) X-ray absorption near-edge spectroscopy investigation of the oxidation state of Pd species in nanoporous SnO2 gas sensors for methane detection. Thin Solid Films 520:909–912View ArticleGoogle Scholar